**HAL Id: hal-00141829**

**https://hal.archives-ouvertes.fr/hal-00141829**

### Submitted on 16 Apr 2007

**HAL is a multi-disciplinary open access**

### archive for the deposit and dissemination of

### sci-entific research documents, whether they are

### pub-lished or not. The documents may come from

### teaching and research institutions in France or

### abroad, or from public or private research centers.

**L’archive ouverte pluridisciplinaire HAL, est**

### destinée au dépôt et à la diffusion de documents

### scientifiques de niveau recherche, publiés ou non,

### émanant des établissements d’enseignement et de

### recherche français ou étrangers, des laboratoires

### publics ou privés.

**Classical nucleation theory in ordering alloys**

**precipitating with L12 structure**

### Emmanuel Clouet, Maylise Nastar

**To cite this version:**

### Emmanuel Clouet, Maylise Nastar. Classical nucleation theory in ordering alloys precipitating with

### L12 structure. Physical Review B: Condensed Matter and Materials Physics (1998-2015), American

### Physical Society, 2007, 75 (13), pp.132102. �10.1103/PhysRevB.75.132102�. �hal-00141829�

## hal-00141829, version 1 - 16 Apr 2007

Emmanuel Clouet∗ _{and Maylise Nastar}

Service de Recherches de M´etallurgie Physique, CEA/Saclay, 91191 Gif-sur-Yvette, France (Dated: April 16, 2007)

By means of low-temperature expansions (LTEs), the nucleation free energy and the precipi-tate interface free energy are expressed as functions of the solubility limit for alloys which lead to the precipitation of a stoichiometric L12 compound such as Al-Sc or Al-Zr alloys. Classical

nu-cleation theory is then used to obtain a simple expression of the nunu-cleation rate whose validity is demonstrated by a comparison with atomic simulations. LTEs also explain why simple mean-field approximation like the Bragg-Williams approximation fails to predict correct nucleation rates in such an ordering alloy.

Since its initial formulation in 1927 by Volmer, We-ber and Farkas and its modification in 1935 by Becker and D¨oring the classical nucleation theory (CNT)1,2,3

has been a suitable tool to model the nucleation stage
in phase transformations. The success of this theory
re-lies on its simplicity and on the few parameters required
to predict the nucleation rate. Recently, the use of
com-puter simulations have allowed to assess the applicability
of the theory for solid-solid phase transformations4,5,6,7_{.}

Thanks to a precise control of simulation conditions, it is possible to get accurate estimations of CNT parameters and thus to make a direct comparison between theory predictions and quantities observed during simulations. One thus gains a deeper understanding of the validity of the different assumptions used by the CNT.

Previous studies have shown that the capillary
approx-imation, which CNT relies on, gives a precise description
of cluster thermodynamics. Within this approximation,
the free energy of a nucleus is written as the sum of a
volume contribution, the nucleation free energy, and a
surface contribution corresponding to the energy cost to
create an interface between the nucleus and the solvent.
For CNT to agree with atomic simulations, care has to
be taken in the way these two energetic contributions
are obtained. In particular, we have shown that one has
to take into account short range order when calculating
the nucleation free energy in an ordering alloy4_{. Usual}

thermodynamic approximations, like the ideal solid
so-lution or the Bragg-Williams approximation, cannot
de-scribe short range order and thus can predict values of
the cluster size distribution and of the nucleation rate
wrong by several orders of magnitude. This is to contrast
with more sophisticated mean-field approximations like
the cluster variation method (CVM) which provides good
predictions of the nucleation rate4_{. However, an easy use}

of CNT and a clear determination of the missing ingre-dients in simple mean-field approximations requires an analytical approach which CVM cannot provide. Such an approach has to lead to accurate expressions of the CNT input parameters so as to make the theory predic-tive without any fitting of its parameters.

In this Letter, we use low-temperature expansions
(LTE)8,9_{to derive an analytical formulation of the }

nucle-ation free energy and the interface free energy in a binary system like Al-Sc or Al-Zr, i.e. a supersaturated Al-X

solid solution leading to the nucleation of a stoichiomet-ric Al3X compound with the L12 structure. This

struc-ture corresponds to an ordering of the fcc lattice with
so-lute X atoms lying on one of the four cubic sublattices8_{.}

LTE are well suited to describe short range order in
dilute solid solution and nearly stoichiometric ordered
compounds10,11,12,13,14 _{like Al}

3X compound. The use of

this method in CNT framework allows to obtain a fully analytical modelling whose only material parameters are the solubility limit and the solute diffusion coefficient.

To do so, we start from the same atomic diffusion
model previously developed for Al-Sc-Zr system4,15_{. This}

model relies on a rigid lattice with interactions between
first- and second nearest neighbors and uses a thermally
activated atom-vacancy exchange mechanism to describe
diffusion. Despite its simplicity, it has been shown to
lead to predictions in good agreement with experimental
data15,16,17_{. Within this atomic model, atoms are }

con-strained to lie on a fcc lattice and the configurations of a binary Al-X alloy is fully described by the solute atom occupation number pn with pn= 1 if the site n is

occu-pied by a solute atom and pn= 0 otherwise. The energy

per atom of a given configuration of the Al-X alloys is then given by E = UAl+ 1 Ns (UX− UAl) X npn + 1 Nsω (1) AlX X′ n,m(1 − pn) pm + 1 Nsω (2) AlX X′′ n,m(1 − pn) pm (1)

where the first and second sums, respectively, run on all first and second nearest-neighbor pairs of sites, Nsis the

number of lattice sites, UAl (respectively UX) is the

en-ergy per atom when only Al (respectively X) atoms lie on the fcc lattice and ω(1)AlX and ω

(2)

AlX are the first and

second nearest neighbor order energies. Sc and
Al-Zr thermodynamics are characterized by the order
ten-dency between first nearest neighbors (ω(1)_{AlX} < 0) and
the demixing tendency between second nearest neighbors
(ω(2)_{AlX}> 0). Eq. 1 is a rewriting for binary alloys of the
atomic model developed in Refs.4,15 _{when one neglects}

2

The nucleation free energy entering CNT is defined by ∆Gnuc(x0X) = 3 4µAl(x eq X) − µAl(x0X) +1 4µX(x eq X) − µX(x0X) , (2)

where µAl(xX) and µX(xX) are the Al and X component

chemical potentials in a solid solution of concentration
xX, and xeq_{X} and x0Xthe concentrations of the equilibrium

and supersaturated solid solution.

LTE are more easy to handle in semi-grand-canonical ensemble where all quantities are written as functions of the effective potential µ = (µAl− µX) /2. Definition of

the nucleation free energy then becomes

∆Gnuc(µ) = A(µeq) − A(µ) +1_{2}(µeq_{− µ) ,} (3)
where µeq_{is the effective potential corresponding to }

equi-librium between the Al solid solution and the Al3X L12

compound. We have defined in Eq. 3 the solid solution semi-grand-canonical free energy A = (µAl+ µX) /2 =

F (x) + (1 − 2x) µ, F (x) being the usual canonical free energy.

A LTE consists in developing the partition function
of the system around a reference state, keeping in the
series only the excited states of lowest energies. Use of
the linked cluster theorem8,9 _{allows then to express the}

corresponding semi-grand canonical free energy as A(µ) = A0(µ) − kTX

i,n

gi,nexp (−∆Ei,n(µ)/kT ), (4)

where the energy of the ground state is A0_{(µ) = U}
Al+ µ

for the Al solid solution and A0(µ) = 3/4 UAl+ 1/4 UX+

3ω_{AlX}(1) + µ/2 for the Al3X L12compound. In the sum

ap-pearing in Eq. 4, the excited states have been gathered according to their energy state i and the number n of lattice sites involved. LTE parameters corresponding to the excited states with the lowest energies are given in Tab. I. All excitation energies only involve a set of iso-lated atoms or in second nearest neighbor position since flipping two atoms at nearest neighbor position produces an excited state with a much higher energy.

The solute concentration in a given phase is obtained
by considering the derivative of the corresponding
semi-grand-canonical free energy. For the solid solution, one
gets
xX(µ) = 1
2
1 −∂A(µ)_{∂µ}
=X
i,n

ngi,nexp (−∆Ei,n(µ)/kT ). (5)

The solid solution and the L12 compound are in

equi-librium when both phases have the same semi-grand canonical free energy. Considering third order LTE

TABLE I: Coefficients entering in the low temperature ex-pansion (Eq. 4). The first seven excited states are considered for the solid solution and the first three excited states for the Al3X L12 compound. The effective potential is written as

µ = (UX− UAl)/2 + 6ω(1)AlX+ δµ.

Solid solution L12 compound

i n ∆Ei,n(µ) gi,n ∆Ei,n(µ) gi,n

1 1 6ω(2)_{AlX}− 2δµ 1 6ω
(2)
AlX+ 2δµ 1/4
2 2 10ω_{AlX}(2) − 4δµ 3 10ω
(2)
AlX+ 4δµ 3/4
3 2 12ω_{AlX}(2) − 4δµ −19/2 12ω
(2)
AlX+ 4δµ −7/8
4 3 14ω_{AlX}(2) − 6δµ 15
5 4 16ω_{AlX}(2) − 8δµ 3
5 3 16ω_{AlX}(2) − 6δµ −96
6 4 18ω_{AlX}(2) − 8δµ 83
6 3 18ω_{AlX}(2) − 6δµ −774
7 5 20ω(2)_{AlX}− 10δµ 48
7 4 + 20ω_{AlX}(2) − 8δµ −1569/2

(i = 3), this happens for the effective potential µeq= (UX− UAl)/2 + 6ω(1)AlX

+3 2kT

h

exp (−6ω(2)AlX/kT ) + 3 exp (−10ω (2) AlX/kT )

−13_{2} exp (−12ω(2)AlX/kT )

, (6) corresponding to the solubility

xeq_{X} = exp_{−6ω}_{AlX}(2) /kT+ 6 exp_{−10ω}(2)_{AlX}/kT
− 16 exp−12ωAlX(2) /kT

. (7) As these expressions have to be consistent with the ex-pansion of A, terms with larger exponential arguments than −12ω(2)AlXare discarded. For equilibrium phases, one

does not need to go further in the expansion than the third order. Indeed, thermodynamic properties are al-ready well converged as the solid solution and the L12

compound in equilibrium only slightly deviate from their respective ground states. On the other hand, Fig. 1 show that an expansion beyond the third order of the semi-grand canonical free energy A(µ) of the supersat-urated solid solution and of the corresponding concen-tration xX(µ) improves the convergence of the

nucle-ation free energy. When only the first excited state
is included in the expansion, LTE leads to the same
value of the nucleation free energy as the ideal solid
solution model. As more excited state are included in
the expansion, the value deduced from LTE converges
to the one calculated with CVM in the
tetrahedron-octahedron approximation4_{. This is to contrast to the}

Bragg-Williams approximation which leads to a worse prediction of the nucleation free energy than the ideal solid solution model.

−60
−40
−20
0
0 0.5 1 1.5
∆
*G*
*nuc*
(meV at.
−1
)
% Zr
CVM
Ideal solid solution
Bragg−Williams
LTE : 1st order
3rd order
7th order

FIG. 1: Variation with the nominal concentration x0

Zr of

the nucleation free energy ∆Gnuc at T = 723 K obtained with different thermodynamic approximations: CVM, ideal solid solution, Bragg-Williams and low-temperature expan-sions (LTE) to different orders.

So as to understand why Bragg-Williams approxima-tion does so bad, it is worth going back to the canonical ensemble. When considering only the third order LTE, thermodynamic quantities can be expressed as functions of the solid solution nominal concentration x0

X. In

par-ticular, the nucleation free energy is given by
∆GnucLTE(x0X) = kTq (x0X) − q (x
eq
X)
+ 3kT exp2ω(2)_{AlX}/kT hq (x0X)
2
− q (xeqX)
2i
−1_{4}kTln q (x0
X) − ln [q (xeqX)] , (8)

where we have defined the function

q (x) = 2x

1 + r

1 + 4xh6 exp2ω_{AlX}(2) /kT_{− 19}i
. (9)

This expression developed to first order in the
concentra-tions x0
X and x
eq
X leads to
∆GnucLTE(x0X) ∼
3
4kT ln
1 − xeqX
1 − x0
X
+1
4kT ln
xeq_{X}
x0
X
+1
4kT
1 + 6e2ω(2)_{AlX}/kT _{x}0
X− xeqX . (10)

Doing the same development for the nucleation
free energy calculated within the Bragg-Williams
approximation4_{, we obtain}
∆GnucBW(x0X) ∼
3
4kT ln
1 − xeqX
1 − x0
X
+1
4kT ln
xeq_{X}
x0
X
+6ω(1)AlX+ 3ω
(2)
AlX
x0X− x
eq
X . (11)

Comparing Eq. 10 with Eq. 11, we see that these two thermodynamic approximations deviate from the ideal solid solution model by a distinct linear term. In the LTE (Eq. 10), the nucleation free energy is only de-pending on the second nearest neighbor interaction and the coefficient in front of the concentration difference is positive. On the other hand, the Bragg-Williams ap-proximation (Eq. 11) incorporates both first and sec-ond nearest neighbor interactions into a global parameter ωAlX= 6ωAlX(1) + 3ω

(2)

AlX. This leads to a linear correction

with a coefficient which can be negative due to the
os-cillating nature of the interactions. In particular, this is
the case for both binary Al-Zr and Al-Sc alloys4_{. }

Bragg-Williams approximation thus leads to a wrong correction of the ideal model because it does not consider properly short range order. In the case of a L12 ordered

com-pound precipitating from a solid solution lying on a fcc
lattice, one cannot use such an approximation to
calcu-late the nucleation free energy. On the other hand, Eq. 8
is a good approximation and can be used to calculate
the nucleation free energy even when the second nearest
neighbor interaction ω(2)_{AlX}is not known. Indeed, this
pa-rameter can be deduced from the solubility limit xeqX by

inverting Eq. 7, leading to the relation
ω_{AlX}(2) = −1
6kT ln (x
eq
X) + kT
xeq_{X}2/3_{−}8
3x
eq
X
. (12)
This relation combined with Eq. 8 provides a powerful
way for calculating the nucleation free energy from the
solid solubility.

LTE can be used too to calculate the plane interface free energy σ100 corresponding to a [100] direction. Due

to the inhomogeneity perpendicular to the interface, the main contribution arises from broken bonds and excited states, whose energies are lower than in bulk phases, only bring a small correction. One thus does not need to go further than the second order in the expansion. At 0 K, the isotropic interface free energy ¯σ is obtained by mul-tiplying σ100 with the geometric factor (6/π)1/3

corre-sponding to a perfect [100] facetting of the precipitates.
For low temperatures, this is a good approximation to
assume that the same linear relation holds between both
quantities4_{. The isotropic interface free energy given by}

LTE is then

a2σ = (6/π)¯ 1/3hω_{AlX}(2) − 2kT exp (−4ωAlX(2) /kT )

−kT exp (−6ωAlX(2) /kT )

i , (13) where a is the fcc lattice parameter.

LTE thus allow to calculate all CNT input parameters from the knowledge of the solubility limit. The nucle-ation rate is then obtained from the equnucle-ation

Jst(x0X) = −16Ns
∆Gnuc_{(x}0
X)
√
kT a2_{σ}_{¯}
DX
a2 x
0
X
exp
−π_{3} (a
2_{¯}_{σ)}3
kT [∆Gnuc_{(x}0
X)]2
, (14)

4
1022
1024
1026
1028
2
1.5
1
0.5
% Zr
*J*
*st* (nuclei m
−3
s
−1
)
*T = 723 K*
*T = 773 K*
*T = 823 K*
*T = 873 K*
*T = 723 K*
*T = 773 K*
*T = 823 K*
*T = 873 K*
1022
1024
1026
1028
1
0.5
% Sc
*J*
*st* (nuclei m
−3
s
−1
)
*T = 723 K*
*T = 773 K*
*T = 823 K*
*T = 723 K*
*T = 773 K*
*T = 823 K*

FIG. 2: Variation with nominal concentration and tempera-ture of the steady-state nucleation rate Jst for Al3Zr (top)

and Al3Sc (bottom) precipitations. Symbols correspond to

kinetic Monte Carlo simulations and lines to classical nucle-ation theory

where DXis the X impurity diffusion coefficient in Al. We

thus obtain a fully analytical expression of the nucleation
rate. Using the same experimental data, i.e. solubility
limits and diffusion coefficients, as the ones used to fit
the atomic diffusion model of kinetic Monte Carlo
simu-lations, we can compare CNT predictions with nucleation
rate observed in simulations4_{. A good agreement is }

ob-tained both for Al-Zr and Al-Sc binary alloys (Fig. 2).

The combination of LTE with CNT thus allows to build a quantitative modeling of nucleation relying on a very limited number of material parameters. Such a model can be directly applied to aluminum alloys where a L12

compound precipitates from a supersaturated solid
so-lution as this is the case with Zr, Sc or other rare earth
elements like Er, Tm, Yb and Lu18_{. Li too precipitates in}

aluminum with a L12structure, but this system requires

another statistical approximation than LTE. Indeed, this approach based on LTE, requires that the precipitating phase only slightly deviates from its perfect stoichiome-try and that the solute solubility remains low. Provided these conditions are fulfilled, it could be applied to al-loys other than aluminum alal-loys. More generally, LTE demonstrate that the oscillating nature of the interac-tions in an alloy with an ordering tendency has to be taken into account by the CNT and requires a better statistical description than the Bragg-Williams approxi-mation which treats all interactions on the same footing.

The authors would like to thank Y. Le Bouar and A. Finel for helpful discussions on LTE, and B. Legrand, F. Soisson and G. Martin for their invaluable help.

∗ _{Electronic address: emmanuel.clouet@cea.fr}

1 _{G. Martin, in Solid State Phase Transformation in }

Met-als and Alloys (Les ´Editions de Physique, Orsay, France, 1978), pp. 337–406.

2 _{K. F. Kelton, in Solid State Physics, edited by H. }

Ehren-reich and D. Turnbull (Academic Press, 1991), vol. 45, pp. 75–177.

3 _{D. Kashchiev, Nucleation : basic theory with applications}

(Butterworth Heinemann, Oxford, 2000).

4 _{E. Clouet, M. Nastar, and C. Sigli, Phys. Rev. B 69,}

064109 (2004).

5 _{V. A. Shneidman, K. A. Jackson, and K. M. Beatty, Phys.}

Rev. B 59, 3579 (1999).

6 _{F. Soisson and G. Martin, Phys. Rev. B 62, 203 (2000).}
7 _{F. Berthier, B. Legrand, J. Creuze, and R. T´etot, J. }

Elec-troanal. Chem. 561, 37 (2004); 562, 127 (2004).

8 _{F. Ducastelle, Order and Phase Stability in Alloys }

(North-Holland, Amsterdam, 1991).

9 _{C. Domb and M. S. Green, eds., Phase Transitions and}

Critical Phenomena, vol. 3 (Academic Press, London,

1974).

10 _{C. Woodward, M. Asta, G. Kresse, and J. Hafner, Phys.}

Rev. B 63, 094103 (2001).

11 _{A. F. Kohan, P. D. Tepesch, G. Ceder, and C. Wolverton,}

Comput. Mater. Sci. 9, 389 (1998).

12 _{M. Asta, S. M. Foiles, and A. A. Quong, Phys. Rev. B 57,}

11265 (1998).

13 _{R. W. Hyland, M. Asta, S. M. Foiles, and C. L. Rohrer,}

Acta Mater. 46, 3667 (1998).

14 _{Y. Le Bouar, A. Loiseau, and A. Finel, Phys. Rev. B 68,}

224203 (2003).

15 _{E. Clouet, L. La´e, T. ´}_{Epicier, W. Lefebvre, M. Nastar, and}

A. Deschamps, Nat. Mater. 5, 482 (2006).

16 _{E. Clouet, A. Barbu, L. La´e, and G. Martin, Acta Mater.}

53_{, 2313 (2005).}

17 _{E. Clouet and A. Barbu, Acta Mater. 55, 391 (2007).}
18 _{K. E. Knipling, D. C. Dunand, and D. N. Seidman, Z.}